The Eshelby, Hill, Moment and Concentration Tensors for Ellipsoidal Inhomogeneities in the Newtonian Potential Problem and Linear Elastostatics
- 1.5k Downloads
- 8 Citations
Abstract
One of the most cited papers in Applied Mechanics is the work of Eshelby from 1957 who showed that a homogeneous isotropic ellipsoidal inhomogeneity embedded in an unbounded (in all directions) homogeneous isotropic host would feel uniform strains and stresses when uniform strains or tractions are applied in the far-field. Of specific importance is the uniformity of Eshelby’s tensor\(\mathbf{S}\). Following Eshelby’s seminal work, a vast literature has been generated using and developing Eshelby’s result and ideas, leading to some beautiful mathematics and extremely useful results in a wide range of application areas. In 1961 Eshelby conjectured that for anisotropic materials only ellipsoidal inhomogeneities would lead to such uniform interior fields. Although much progress has been made since then, the quest to prove this conjecture is still not complete; numerous important problems remain open. Following a different approach to that considered by Eshelby, a closely related tensor \(\mathbf{P}=\mathbf{S}\mathbf{D}^{0}\) arises, where \(\mathbf{D}^{0}\) is the host medium compliance tensor. The tensor \(\mathbf{P}\) is associated with Hill and is of course also uniform when ellipsoidal inhomogeneities are embedded in a homogeneous host phase. Two of the most fundamental and useful areas of applications of these tensors are in Newtonian potential problems such as heat conduction, electrostatics, etc. and in the vector problems of elastostatics. Knowledge of the Hill and Eshelby tensors permit a number of interesting aspects to be studied associated with inhomogeneity problems and more generally for inhomogeneous media. Micromechanical methods established mainly over the last half-century have enabled bounds on and predictions of the effective properties of composite media. In many cases such predictions can be explicitly written down in terms of the Hill tensor, or equivalently the Eshelby tensor and can be shown to provide excellent predictions in many cases.
Of specific interest is that a number of important limits of the ellipsoidal inhomogeneity can be taken in order to be employed in predictions of the effective properties of, for example, layered media and fibre reinforced composites and also to the cases when voids and cracks are present. In the main, results for the Hill and Eshelby tensors are distributed over a wide range of articles and books, using different notation and terminology and so it is often difficult to extract the necessary information for the tensor that one requires. The case of an anisotropic host phase is also frequently non-trivial due to the requirement of the associated Green’s tensor. Here this classical problem is revisited and a large number of results for problems that are felt to be of great utility in a wide range of disciplines are derived or recalled. A scaling argument leads to the derivation of the Eshelby tensor for potential problems where the host phase is at most orthotropic, without the requirement of using the anisotropic Green’s function. The Concentration tensor \(\boldsymbol{\mathcal{A}}\) linking interior fields to those imposed in the far-field is derived for a wide variety of problems. These results can therefore be used in the various micromechanical schemes.
Directly related to the tensors of Eshelby and Hill is the so-called Moment tensor \(\mathbf{M}\). As well as arising in the literature on micromechanics, this tensor is important in the vast area of research associated with inverse problems and specifically with the problem of identifying an object inside some domain given the application of a specific set of boundary conditions. Due to its fundamental importance and direct link to the Eshelby and Hill tensors, here we state the connection between \(\mathbf{M}, \mathbf{P}\) and \(\mathbf{S}\) in an effort to ensure that the work is of use to as wide a community as possible.
Both tensor and matrix formulations are considered and contrasted throughout. Appendices give various details that illustrate the implementation of both approaches.
Keywords
Hill tensor Eshelby tensor Moment tensor Concentration tensor Newtonian potential Elastostatics Eshelby conjecture Pólya-Szegö conjecture Inclusion Inhomogeneity Ellipsoids Uniformity Micromechanics Homogenization Inverse problems Elastic modulus tensor Conductivity tensorMathematics Subject Classification
31B05 31B10 31B20 31B35 35C15 35J05 35J08 35J15 35J25 35R05 45A05 74A40 74A60 74B05 74E05 74E10 74E30 74E35 74G05 74G70 74G75 74L10 74M25 74N15 74Q05 74Q15 78A30 78M40 80A20 80M401 Introduction
The canonical isolated inhomogeneity problem has been of fundamental importance in a number of materials modelling problems now for well over a century. This problem is the following: a single inhomogeneity or particle of general shape, with different material properties to that of the surrounding material is embedded inside an unbounded (in all directions, i.e., free-space) homogeneous host medium. Given some prescribed conditions in the far-field, what form do the fields take within the inhomogeneity? As well as being interesting in its own right, this problem is of utmost importance in homogenization, micromechanics and multiscale modelling.
The first to consider this kind of inhomogeneity problem was Poisson in 1826 [103] who studied the perturbed field due to an isolated ellipsoid in the context of the Newtonian potential problem. He showed that given a uniform electric polarization (or magnetization), the induced electric (or magnetic) field inside the ellipsoid is also uniform. In 1873 Maxwell [83] derived explicit expressions for this field. Early work in linear elasticity saw a number of studies determine the field inside and around inhomogeneities, including the important case of a cavity (since this was correctly recognized as a defect or flaw). Examples of these works are those associated with the case of spheres [43, 118], spheroids [29] and ellipsoids [107, 113, 114] but all considered specific loadings, usually of the homogeneous type in the far-field, meaning uniform tractions or displacements that are linear in the independent Cartesian variable, say \(\mathbf{x}\).
The inhomogeneity problem is now usually associated with the name of Eshelby because in 1957 he showed that for general homogeneous conditions imposed in the far-field, the strain set up inside an isotropic homogeneous ellipsoid is uniform [31]. In 1961 Eshelby [32] conjectured that “…amongst closed surfaces, the ellipsoid alone has this convenient property…”. One could ask is this really true? In the sense of what it is thought that Eshelby meant when he made this conjecture (the so-called weak Eshelby conjecture, where the interior field must be uniform for any homogeneous far-field loading), this statement certainly is true although this was only proved in 2008, simultaneously by Kang and Milton [56] and Liu [71] in the case of isotropic media. There is a slightly different version (the so-called strong Eshelby conjecture), where the interior field must be uniform only for a specific, single uniform far-field loading. This strong conjecture has not been proven in the context of three dimensional isotropic linear elasticity, although significant progress has been made in the last decade, see [55] for a review. The results obtained in [4] go beyond the weak Eshelby conjecture but still do not fully prove the strong conjecture. Interestingly the weak conjecture for the associated Newtonian potential problem was proved some time before Eshelby’s 1957 elastostatics paper, by Dive in 1931 [24] and Nikliborc [97] in 1932, see also the discussion in [55, 56, 71]. In deriving these results, Dive and Nikliborc proved the converse of Newton’s theorem that if \(V_{1}\) is an ellipsoid of uniform density, the gravitational force in \(V_{1}\) is zero [58]. The strong conjecture in the context of the potential problem is true in two dimensions [111, 115] but is not true in dimensions greater than two: a non-ellipsoidal counterexample associated with a specific far-field loading (equivalently a specific eigenstress) was found by Liu [71].
It is important to note that the proofs of Eshelby’s conjectures in elastostatics referred to above correspond to simply connected, isotropic inhomogeneities with Lipschitz boundaries. Eshelby’s work was followed up by numerous researchers who considered the general anisotropic case [6, 8, 32, 61, 70, 121, 122, 129, 133]. In 1974 Cherepanov [22] proved that multiple inhomogeneities of non-ellipsoidal shape can interact in order to render the interior fields uniform; see also Kang and Milton [56] and Liu [71] who coined the term E-inclusions for such interacting inhomogeneities. Liu and co-workers have also considered the periodic Eshelby problem in two dimensions [72, 73]. Kang and Milton [56] used their approach to prove Eshelby’s weak conjecture in the context of the fully anisotropic potential problem. Most notably however, it is stressed again that the weak Eshelby conjecture for elasticity has not yet been proved in the context of anisotropic elasticity.
Interest in deriving the Eshelby tensor for non-ellipsoidal inhomogeneities has always been active in order to show that the conjecture holds for specific classes of inhomogeneities. Particular attention has been paid to polygonal and polyhedral inhomogeneities and the associated properties of Eshelby’s tensor [57, 74, 79, 80, 93, 94, 98, 108]. The supersphere case has been considered recently by [18] building on the work by [99, 100, 119]. A general method was developed by Ru [110] in order to obtain an analytical solution associated with a two dimensional inhomogeneity of arbitrary cross section and explicit forms of the stress inside hypotrochoidal and rectangular inhomogeneities were derived. Some analytical expressions have recently been derived for two-dimensional problems in the Newtonian potential and plane elastostatics problems where inhomogeneities are either polygonal or their shape can be described by finite Laurent expansions [140, 141]. Additional useful properties of the Eshelby tensor have been deduced, including the relationship of the averaged Eshelby tensor for non-ellipsoidal inhomogeneities to their ellipsoidal counterparts [126, 137].
More recently the inhomogeneity problem has been studied in the nonlinear elasticity context where results associated with Eshelby’s conjecture have been proved in two dimensions for so-called harmonic materials [59, 60, 112]. Although nonlinear problems are generally more difficult than linear elastostatics, the nonlinearity frees up a number of issues that are more constrained in linear problems. The study of nonlinear problems with dilatational eigenstrain was recently carried out in [135]. Giordano [41] considered the nonlinearly elastic inhomogeneity problem but where the constitutive behaviour is described via expansions in strain (Landau elasticity).
The Hill and Eshelby tensors are of great utility in a number of micromechanical methods and what is quite astonishing is that they can be evaluated analytically in a large number of very important cases. However, results are distributed over a large number of articles, reviews and textbooks, and furthermore often in articles that span a wide range of scientific fields due to the wide ranging applicability of the theory. References dealing with derivations of specific results are those of [10, 14, 28, 81, 106, 123, 132] and [67]. The field is still very much alive, pushed forward by both unresolved theoretical issues as well as applications involving not only inhomogeneities but also cracks and dislocations [95, 139] and by the desire to fully resolve the open issues described above. Recent work has focused in more detail on inhomogeneities of general shape and how these can feed into models of inhomogeneous media with distributions of non-canonical inhomogeneities [14, 15, 16, 33, 34, 35, 138, 140, 141]. Such studies are important to understand how local stress fields develop in the medium under loading. This is highly dependent upon the inhomogeneity shape. It must always be stressed that the utility of the Eshelby tensor itself for general shapes in micromechanical methods is limited by the fact that fields interior to the inhomogeneity are not generally uniform in such cases and therefore the tensor does not arise as a natural quantity from the governing integral equations ((2.7) and (2.11) below) as it does in the case of ellipsoidal inhomogeneities.
Here the objective is to gather together important results associated with the Hill and Eshelby tensors for ellipsoidal inhomogeneities in a consistent notation, derive a number of important limiting cases such as those associated with cracks and cavities, derive compact results associated with the anisotropic potential problem and finally derive and state associated Concentration tensors. This should prove useful to many who frequently require the form of the \(\mathbf{P}\)- or \(\mathbf{S}\)-tensors in practice but who struggle to find the appropriate reference. The emphasis here is to derive the Hill, Eshelby and Concentration tensors but as is clear from (1.3) the Moment tensor follows straightforwardly from these.
An important point to note is that using the so-called invariant notation, potential and linear elastostatics problems can be considered simultaneously, only that the latter is a higher order tensor analogue of the former. Here however the applications are made distinct in order to stress the different results and mechanisms for deriving these expressions. In particular the results from potential theory feed into those from linear elastostatics. As a result, index notation shall be used almost entirely throughout.
In much of the literature on micromechanics the terms inclusion and inhomogeneity are used interchangeably. However in some cases they are used to make an important distinction. An inhomogeneity is defined as a particle of general shape having different material properties to those of the surrounding medium in which it is embedded. On the other hand the terminology inclusion is used to represent a general shaped region within some medium that has the same properties as the surrounding medium but where this finite inclusion region has been subject to some eigenstrain (e.g., thermal strain). This differentiation is used, e.g., in Mura [92] and Qu and Cherkaoui [106] and it is also adopted here.
In Sect. 2 the integral equation formulation of the inhomogeneity problem is stated, yielding integral equations for the potential gradient and strain inside an inhomogeneity. In Sect. 3 it is illustrated that such fields are uniform when the inhomogeneity is ellipsoidal and the general expressions for the associated Hill tensors are stated. The notion of Concentration tensors is also discussed. In Sects. 4 and 5 specific results are then stated and derived for the cases of the Newtonian potential problem and elastostatics respectively. A closing discussion is given in Sect. 6 describing how the results are used in micromechanical methods together with a summary of current areas of associated research. Numerous important details and results are stated in Appendices in order for this review to be comprehensive but also to aid the flow of reading, in particular the mechanism for representing tensors of certain symmetries with respect to appropriate tensor bases, tensor contractions, and the matrix formulation of operations between tensors are covered in Appendix C.
As many pertinent references are given as possible; it is important to stress that the focus is specifically on the formulation of the Eshelby, Hill and Concentration tensors rather than articles associated with micromechanical methods, of which there are thousands. For the latter the interested reader is referred to the many textbooks that have been written over the last decade, e.g., [14, 28, 54, 67, 106].
2 Integral Equation Formulation
Index notation shall be used for tensors throughout, working in Cartesian coordinates and using repeated subscripts to imply summation. The term unbounded will be used when referring to free-space, i.e., unbounded in all directions. Although a general invariant formulation can be employed to deal with problems in the potential and linear elastostatics context simultaneously [132], this approach can obfuscate details that are important when it comes to deriving specific Hill and Eshelby tensors for given anisotropies and inhomogeneity shapes, which is the main purpose of this article.
2.1 The Potential Problem
2.2 Elastostatics
The origins of the \(\mathbf{P}\)-tensor reside in the context of elastostatics rather than in potential problems even though the theory is of course analogous. The \(\mathbf{P}\)-tensor originated with Hill [47] who also introduced the compact notation (now commonly referred to as Hill notation) for transversely isotropic fourth order tensors, which is summarized in Appendix C.2.3. Walpole [122], Willis [130, 131, 132] and Laws [62] amongst others followed this with influential work associated with inhomogeneities of specific shapes, paying particular attention in many cases to the scenarios of discs, fibres and cracks. A number of \(\mathbf{P}\)-tensors are also stated in the excellent concise review of micromechanics by Markov [81] although unfortunately, some typographical errors are present there and these are corrected here.
3 Uniformity of the Hill and Eshelby Tensors
3.1 The Potential Problem
Clearly since the integral is over the surface of the unit sphere \(S^{2}\), it is sensible to resolve \(\overline{\xi}_{i}\) into spherical polar coordinates for the purposes of evaluating this integral. The form of (3.3) illustrates the important general result that the \(\mathbf{P}\)-tensor is uniform for an arbitrarily anisotropic ellipsoidal inhomogeneity embedded inside an arbitrarily anisotropic host phase. That Eshelby’s (weak) conjecture is true for anisotropic potential problems [56, 71], means that the ellipsoid is the only shaped inhomogeneity for which the interior temperature gradient is uniform under any such far-field condition of the form (3.1). The fact that the strong conjecture is not true in the Newtonian potential problem means that there exists shapes where the interior temperature gradient field can be uniform for specifically chosen homogeneous far-field conditions [71].
To determine the appropriate \(\mathbf{P}\)-tensor in any circumstance then one can appeal to (3.3) and carry out the necessary integration. Alternatively, as shall be shown in Sect. 4, in many cases it is relatively straightforward to use symmetry arguments and results from potential theory in the isotropic host case together with scalings in some cases of host anisotropy, in order to derive explicit results, often in a more straightforward manner than by directly evaluating the general expression (3.3). In fact in the potential problem context, symmetry arguments and results from potential theory [58] are often sufficient to derive results for many special cases of ellipsoids in host media that are at most orthotropic. The general result (3.3) is thus suitable for more complex anisotropies than orthotropy or for example if the semi-axes of the ellipsoid are not aligned with the axes of symmetry of host anisotropy.
In the host region \(V_{0}\) the temperature gradient is generally not uniform.
For non-homogeneous temperature gradient conditions in the far-field, the temperature gradient field inside an ellipsoidal inhomogeneity is generally not uniform. However if the prescribed temperature gradient is a polynomial of order \(n\), then so is the field inside an ellipsoidal inhomogeneity, see [6]. This is known as the polynomial conservation property for ellipsoids.
Generally for non-ellipsoidal inhomogeneities in unbounded domains and general shaped inhomogeneities in bounded host domains \(V\), the temperature gradient inside the inhomogeneities is not uniform, although interacting E-inclusions [71] can lead to uniform interior temperature gradients and for specific loadings, non-ellipsoidal inhomogeneities can yield uniform interior temperature gradients, e.g., the counterexample of the Strong Eshelby conjecture given by Liu [71].
3.2 Elastostatics
That Eshelby’s (weak) conjecture is true for isotropic elastostatics problems [56, 71], means that the ellipsoid is the only shaped inhomogeneity for which the interior temperature gradient is uniform under any such far-field condition of the form (3.7). It is stressed however that it is not yet clear whether the weak conjecture is true in the context of anisotropic problems.
To determine the \(\mathbf{P}\)-tensor for an ellipsoid for a given host anisotropy one merely has to evaluate the surface integral in (3.9) and this can be done numerically very efficiently. For host anisotropies more complex than transversely isotropic it is generally recommended that the form (3.9) be employed and integrals are evaluated numerically. In what follows here the \(\mathbf{P}\)-tensor shall be determined in the case of an isotropic host phase by appealing to various symmetries and potential theory. An important result derived by Withers [133] associated with a transversely isotropic host phase is also stated.
3.3 The Potential Gradient Tensor and Strain Concentration Tensor
Note that \(\mathcal{A}_{ij}\) is the Concentration tensor associated with an isolated inhomogeneity inside an unbounded host medium. The calligraphic notation \(\mathcal{A}_{ij}\) has been used to stress the link with (and distinguish from) the exact Concentration tensor whose components are usually defined as \(A_{ij}\), and which links the phase average of the true temperature gradient inside an inhomogeneity to that in the far-field in a complex inhomogeneous medium, which may consist of interacting inhomogeneities. For a dilute medium where interaction effects can be neglected, \(A_{ij}=\mathcal{A}_{ij}\).
4 The Potential Problem: Specific Cases
4.1 Isotropic Host Phase
Once \(P_{ij}\) is determined for an isotropic host phase the associated Concentration tensor for an isolated inhomogeneity may then be found from (3.19) as is now illustrated in a number of special cases of specific inhomogeneities with given shape and anisotropy.
4.1.1 Sphere in an Isotropic Host Phase
Isotropic Sphere
Anisotropic Sphere
4.1.2 Circular Cylinder in an Isotropic Host Phase
4.1.3 Ellipsoid in an Isotropic Host Phase
4.1.4 Spheroid in an Isotropic Host Phase
- (i)
a sphere, i.e., \(\varepsilon \rightarrow1\), it is deduced that \(\gamma =\gamma _{3} = \frac{1}{3}\),
- (ii)
a cylinder, i.e., \(\varepsilon \rightarrow\infty\), it is deduced that \(\gamma _{3}= 0\), \(\gamma =\frac{1}{2}\),
- (iii)
a disc or layer, i.e., \(\varepsilon \rightarrow0\), it is deduced that \(\gamma _{3}=1\), \(\gamma =0\).
4.1.5 Limiting Case of an Elliptical Cylinder
4.1.6 Limiting Cases of a Cavity, Penny-Shaped Crack and Ribbon-Crack
It does not make sense to define a temperature gradient Concentration tensor in the context of cracks or cavities because clearly there is no interior field. However it turns out that this concept is useful and can be interpreted as linking the far-field to the field on the surface of such inhomogeneities [50] with an appropriate definition of cavity temperature gradient. Here the results above are used in order to derive associated Concentration tensors for cracks and cavities.
The coefficient of \(\delta_{i3}\delta_{j3}\) in (4.40) involves an apparently singular limit as \(\varepsilon \rightarrow0\). That this is not a problem arises from the fact that this expression is used in formulae for effective properties of cracked media where this term is always multiplied by a volume-fraction term (or rather a crack-density term) that is proportional to \(\varepsilon \) [48, 49]. Note that taking the limits in the opposite order, i.e., \(\varepsilon \rightarrow0\) and then\(k_{1}\rightarrow0\) yields an inconsistent result, giving rise to singular effective material behaviour in the crack limit, which cannot be correct.
4.2 Anisotropic Host Phase
The general form (3.3) for the \(\mathbf{P}\)-tensor associated with arbitrary host anisotropy requires the necessary surface integral to be evaluated. In the case of transversely isotropic and orthotropic media however, where principal axes are aligned with the semi-axes of the ellipsoid, the problem can be simplified significantly by employing a scaling of the Cartesian variables in order to reduce the isolated ellipsoidal inhomogeneity problem in an anisotropic medium to the case of an ellipsoidal inhomogeneity (with different semi-axes) in an isotropic medium. Therefore the results derived above for the isotropic host phase case can be used in the scaled domain and then mapped back to the physical domain in order to obtain the appropriate physical Hill and Eshelby tensors.
4.2.1 Spheroid in a Transversely Isotropic Host Phase
4.2.2 Circular Cylinder in a Transversely Isotropic Host Phase
An interesting non-standard example is the case of a spheroid embedded inside a transversely isotropic host phase where the axes of symmetry and semi-axes are not coincident. In this case the general (surface integral) form of the \(\mathbf{P}\) and \(\mathbf{S}\)-tensors must be used with the semi-axes aligned with the \(\mathbf{x}\) axes but with all components of the modulus tensor being generally non-zero.
4.2.3 Ellipsoid in an Orthotropic Host Phase
Summary of results for the \(\mathbf{P}\)-tensor associated with ellipsoidal inhomogeneities for potential problems
Host anisotropy | Inhomogeneity shape | P-tensor |
---|---|---|
Isotropic | Ellipsoid \(a_{1}\neq a_{2}\neq a_{3}\) \(\varepsilon _{n}=a_{3}/a_{n}\) | Use potential theory: \(P_{ij} = \frac{1}{k_{0}}\sum_{n=1}^{3}\mathcal{E}(\varepsilon _{n};\varepsilon _{1},\varepsilon _{2})\delta_{in}\delta_{jn}\) |
Spheroid \(a_{1}=a_{2}=a\neq a_{3}\) \(\varepsilon =a_{3}/a\) | Use potential theory: \(P_{ij} = \frac{1}{k_{0}} (\gamma \varTheta_{ij}+\gamma _{3}\delta_{i3}\delta _{j3} )\) \(\gamma =\frac{1}{2}(1-\gamma _{3}), \gamma _{3} = \mathcal{S}(\varepsilon )\) | |
Sphere | Use symmetry: \(P_{ij} = \frac{1}{3k_{0}}\delta_{ij}\) | |
Transversely isotropic \(\upsilon_{1}=\upsilon_{2}=1\neq\upsilon_{3}=\upsilon\) | Ellipsoid \(a_{1}\neq a_{2}\neq a_{3}\) \(\varepsilon _{n}=a_{3}/a_{n}\) | Use scalings and potential theory: \(P_{ij} = \frac{1}{k_{0}}\sum_{n=1}^{3}\frac{1}{\upsilon_{n}}\mathcal {E}(\hat{\varepsilon }_{n}; \hat{\varepsilon }_{1},\hat{\varepsilon }_{2})\delta_{in}\delta_{jn}\) \(\hat{\varepsilon }_{n} = \hat{a}_{3}/\hat{a}_{n}\) and \(\hat{a}_{n} = a_{n}/\sqrt {\upsilon_{n}}\) |
Spheroid \(a_{1}=a_{2}=a\neq a_{3}\) and \(a_{3}\) is aligned with axis \(x_{3}\) of transverse isotropy | Use scalings and potential theory: \(P_{ij} = \frac{1}{k_{0}} (\gamma \varTheta _{ij}+\gamma _{3}\delta_{i3}\delta_{j3} )\) \(\gamma =\frac{1}{2}(1-\upsilon \gamma _{3})\), \(\gamma _{3} = \frac{1}{\upsilon }\mathcal{S} (\frac{\varepsilon }{\sqrt {\upsilon}} )\) | |
Sphere | Special case of spheroid result above: \(P_{ij} = \frac{1}{k_{0}} (\gamma \varTheta_{ij}+\gamma _{3}\delta_{i3}\delta _{j3} )\) \(\gamma =\frac{1}{2}(1-\upsilon \gamma _{3}), \gamma _{3} = \frac{1}{\upsilon }\mathcal{S} (\frac{1}{\sqrt{\upsilon}} )\) | |
Orthotropic \(\upsilon_{1}=1\neq\upsilon_{2}\neq\upsilon_{3}\) | Ellipsoid \(a_{1}\neq a_{2}\neq a_{3}\) | Use scalings and potential theory: \(P_{ij} = \frac{1}{k_{0}}\sum_{n=1}^{3}\frac{1}{\upsilon_{n}}\mathcal {E}(\hat {\varepsilon }_{n};\hat{\varepsilon }_{1},\hat{\varepsilon }_{2})\delta_{in}\delta _{jn}\) \(\hat{\varepsilon }_{n} = \hat{a}_{3}/\hat{a}_{n}\) and \(\hat{a}_{n} = a_{n}/\sqrt {\upsilon_{n}}\) |
Worse than orthotropic or semi-axes of ellipsoids not aligned with axes of anisotropy | Use general integral form: \(P_{ij}=\frac{\mathrm {det}(\mathbf{a})}{4\pi} \int _{S^{2}}\frac {\varPhi_{ij}\,dS(\overline{\boldsymbol{\xi }})}{(\overline{\xi}_{k} a_{k\ell}a_{\ell m}\overline{\xi }_{m})^{3/2}}\) \(\varPhi_{ij}= \overline{\xi}_{i}\overline{\xi}_{j}/(C_{k\ell }^{0}\overline{\xi}_{k}\overline{\xi}_{\ell})\) |
5 Elastostatics: Specific Cases
5.1 Isotropic Host Phase
Once \(P_{ijk\ell}\) is determined, the components of the Eshelby tensor can be calculated from (1.2) and the associated Concentration tensor can be found from (3.23). Recall that no assumptions have been made regarding the anisotropy of the inhomogeneity. This is not required in order for the \(\mathbf{P}\)-tensor to be determined. The only aspects of the inhomogeneity that influence the \(\mathbf{P}\)-tensor are its shape and, for anisotropic host phases, its orientation with respect to the axes of anisotropy of the host phase.
5.1.1 Sphere in an Isotropic Host Phase
Isotropic Sphere
Cubic Sphere
5.1.2 Circular Cylinder in an Isotropic Host Phase
Short-hand notation for contractions of the basis tensors \(\mathcal {H}_{ijkl}^{n}\)
\(\mathcal{H}^{1}\) | \(\mathcal{H}^{2}\) | \(\mathcal{H}^{3}\) | \(\mathcal{H}^{4}\) | \(\mathcal{H}^{5}\) | \(\mathcal{H}^{6}\) | |
---|---|---|---|---|---|---|
\(\mathcal{H}^{1}\) | \(\mathcal{H}^{1}\) | \(\mathcal{H}^{2}\) | 0 | 0 | 0 | 0 |
\(\mathcal{H}^{2}\) | 0 | 0 | 2\(\mathcal{H}^{1}\) | \(\mathcal {H}^{2}\) | 0 | 0 |
\(\mathcal{H}^{3}\) | \(\mathcal{H}^{3}\) | 2\(\mathcal{H}^{4}\) | 0 | 0 | 0 | 0 |
\(\mathcal{H}^{4}\) | 0 | 0 | \(\mathcal{H}^{3}\) | \(\mathcal{H}^{4}\) | 0 | 0 |
\(\mathcal{H}^{5}\) | 0 | 0 | 0 | 0 | \(\mathcal{H}^{5}\) | 0 |
\(\mathcal{H}^{6}\) | 0 | 0 | 0 | 0 | 0 | \(\mathcal{H}^{6}\) |
5.1.3 Spheroid in an Isotropic Host Phase
5.1.4 Elastic Layer
5.1.5 Limiting Case of a Penny-Shaped Crack
The case of an ellipsoid in an isotropic medium shall now be considered. In order to deal with this generally in a tensor setting, ideally an orthotropic tensor basis should be used. Although it is possible to write down such a basis, details are rather lengthy and in fact for practical computation, it is perhaps most sensible to write down the nine independent components of the \(\mathbf{P}\)-tensor and use matrix computations in the manner described after Sect. 5.1.2 above.
5.1.6 Ellipsoid in an Isotropic Host Phase
The nine independent components of the \(\mathbf{P}\)-tensor for an ellipsoid can be defined in terms of the function \(\mathcal{E}(\varepsilon _{n};\varepsilon _{1},\varepsilon _{2})\) and the semi-axes ratios \(\varepsilon _{n}\).
5.1.7 Elliptical Cylinder and Ribbon-Crack Limit
5.1.8 Flat Ellipsoid
5.1.9 Spheroid Limit Check
5.2 Anisotropic Host Phase
In the potential problem case, scaling coordinate systems assisted in the derivation of results associated with anisotropic media. Although such methods can sometimes lead to modest simplifications in elasticity, the general theory does not lead to any significant advances, certainly for the problems that are of greatest interest in micromechanics. In particular such methods do not lead to significant simplifications for generally transversely isotropic media which is a material symmetry of great importance. Therefore to derive the \(\mathbf{P}\)-tensors associated with inhomogeneities in anisotropic host phases, it is best to work with the integral form of the \(\mathbf{P}\)-tensor as defined in (3.9) for an ellipsoid.
Few explicit results are available in general however since the Green’s tensor cannot generally be determined analytically. One of the few that can be determined is that associated with transversely isotropic media. Withers derived the associated Eshelby tensor for a spheroid [133] using the form of the Green’s function determined by Pan and Chou [101] and we state his result here where the semi-major or minor axis of the spheroid is aligned with the axis of transverse isotropy. This result shall then be validated by employing the general integral form (3.9). Only in the last decade have articles started to appear that compute effective properties of composite media with anisotropic inhomogeneities via micromechanical methods (e.g., [42, 116]). It is also important to note specific results for the Eshelby and Hill tensors associated with cracks in anisotropic media, e.g., Gruescu et al. [44] and Barthélémy [9].
5.2.1 Spheroid in a Transversely Isotropic Host Phase
Derivation from Withers’ Eshelby Tensor
Derivation from the Direct Integral Form
Concentration Tensor
Alternatively suppose that the inhomogeneity is transversely isotropic with the same symmetry axis as the host so that it possesses the elastic modulus tensor of the form (5.145) but where now the constants \(c^{1}_{n}\) are defined in terms of the 5 independent components of this tensor. Then the Concentration tensor is again defined by (5.151) but of course now with the \(c^{1}_{n}\) associated with the transversely isotropic cylinder. This indicates the merit of using the above notation since one can still use (5.151)–(5.153) in this case, merely modifying the \(c^{1}_{n}\) to account for the transverse isotropy of the cylinder.
As usual, the matrix form of these fourth order tensors can be employed for computational efficiency when the problems lack simple symmetries.
5.2.2 Circular Cylinder in a Transversely Isotropic Host
6 Discussion
6.1 Association with Micromechanics
Many micromechanical methods use a more sophisticated approximation that can account, in an approximate manner at least, for interactions. One of the most commonly employed methods is the so-called classical self consistent method [54]. Interaction is approximated in this most simple self-consistent scheme by taking the host medium in the determination of \(\boldsymbol{\mathcal{A}}\) to be the unknown effective medium. In general then (6.1) gives rise to a nonlinear system of equations for the determination of effective properties. In many cases these are not even algebraic equations. Furthermore for the self consistent method, one has to make an assumption in advance of the symmetry properties of the effective tensor. For example in the case of aligned spheroids \(\mathbf{C}^{*}\) will be transversely isotropic.
The textbooks referred to at the end of Sect. 1 provide an excellent introduction to the numerous micromechanical methods, many of which are based on the form of effective modulus tensor defined in (6.1). A similar form can be deduced for media where there is no distinguishable host phase (for example the case of polycrystals) and also for media where multiphysics effects are important as described in the next section.
6.2 Beyond the Potential Problem and Elastostatics
A large number of explicit, compact results associated with the Hill and Eshelby tensors for ellipsoidal inhomogeneities, as well as their associated Concentration tensors have been collected, stated and in some cases derived. The intention is that this will be of great utility to a large number of researchers for implementation in micromechanical and bounding schemes. A thorough discussion of both matrix and tensor (where possible due to space limitations) formulations has been carried out. Typographical errors in past articles and reviews have been corrected and a common notation has been employed.
Although the general integral forms (3.3) and (3.9) are useful they should generally be avoided where explicit forms are available. Gavazzi and Lagoudas [40] described a numerical implementation for elasticity. It should be noted that recently Masson [82] derived a new form of the \(\mathbf{P}\)-tensor in terms of a single integral, although the integrand is inevitably more complex than that in the surface integral in (3.9).
In the literature many of the cases described above are considered as approximations to more complicated shaped inhomogeneities. In terms of the derivation of overall effective properties this is extremely useful, certainly as a first approximation, since it avoids complex computational simulations. However it must be stressed that more advanced analysis is required if detailed micromechanical information such as stress concentration calculations close to inhomogeneities of a complex shape is required [15]. For finite domains, provided the host phase is in some sense much larger than the inhomogeneity, if the inhomogeneity is ellipsoidal then the temperature gradient or strain field inside the ellipsoid is well approximated as being uniform. The inhomogeneity problem associated with bounded domains is described in the book by Li and Wang [67] which summarizes the work in [68, 69].
Continuing with discussion associated with the potential problem and elastostatics first, an important extension of the inhomogeneity problem is that of the coated inhomogeneity. This problem is popular, not least because it arises as a micromechanics problem in the generalized self-consistent method (GSCM) [23]. The so-called double inclusion problem dates back many decades and was solved approximately by Hori and Nemat-Nasser [50] although the approximations involved lead to some rather counter-intuitive predictions when used in the GSCM [51]. Exact solutions in the case of concentric spheroids or ellipsoids have been derived by Hatta and Taya [46] in the thermal context and Jiang et al. [52] in two-dimensional elasticity. See also [75, 76] for elasticity problems involving coated spheres and cylinders respectively. The case of inhomogeneities with radially dependent material properties has been considered in Chap. 3 of [54] amongst others. The coated inhomogeneity is also of interest due to its association with the neutral inclusion problem [89]. Associated with the coated inhomogeneity is the scenario when the interface of an inhomogeneity with the host phase is imperfect [37, 63]. This imperfection can itself be used as the basis for a neutral inclusion [12, 109]. Moment tensors have recently been discussed in the context of cloaking [5].
It is important to note that when the inhomogeneity becomes very small, i.e., the case of a nano-inhomogeneity, then surface energies become non-negligible. This problem has been considered by Sharmi and Ganti [117] and Duan et al. [25] for example. Including surface energies is important in order to incorporate size-dependent effects in effective properties. These are absent in classical micromechanical methods that use the standard Eshelby or Hill tensors.
Eshelby’s problem has also been considered in the context of micro-continuum elasticity models, which themselves were introduced in order to bridge the gap between continuum and atomistic/molecular models [30]. Micropolar (Cosserat) theory has been considered by Cheng and He [20, 21] and Ma and Hu [77]. Micro-stretch theory has been developed by Ma and Hu [78]. Strain gradient constitutive behaviour was studied by Gao and Ma [38, 39].
The dynamic problem was considered for spheres and cylinders by Mikata and Nemat-Nasser [87, 88] and more generally in [19, 84]. Rate dependence of the Hill and Eshelby tensors has been considered by Suvarov and Dvorak [120] and viscoelastic properties have been studied by Wang and Weng [125] by using transform techniques and correspondence principles. Nguyen et al. [96] studied cracked viscoelastic solids using the appropriate Eshelby tensor. Extensions to plasticity have been considered, see [36, 53, 64] for example.
The Newtonian potential and elastostatics problems are canonical problems that can assist with the development of coupled (multiphysics) problems. Dunn and Taya [26], Dunn and Wienecke [27] and Mikata [85, 86] considered the case of piezoelectricity and the prediction of the electroelastic moduli. Li and Dunn [66] and Zhang and Soh [136] considered full coupling and the resulting effective moduli associated with piezoelectromagnetic media. The theory associated with poroelastic and thermoelastic behaviour was developed by Berryman [11] and extended to the anisotropic case by Levin and Alvarez-Tostado [65].
Upon closing it should be noted that it is very fortuitous that such elegant and concise uniformity results hold for ellipsoidal inhomogeneities. These results allow a large number of expressions to be derived analytically and therefore the results have been utilized a great deal. Having said that there is much work to be done. As has been noted, the Eshelby conjecture is still not fully resolved [4], analysis for general shaped inhomogenities continues [16], specifically in the context of stress analysis and resulting effective properties and although computational methods are powerful, they are still only able to solve elasticity problems for inhomogeneous media with an order of 1000 inhomogeneities in “reasonable” times. For use in Monte-Carlo schemes this is therefore still computationally expensive. Nonlinear problems in the context of finite elasticity still require attention [135] and this applies to coupled problems as well.
Footnotes
- 1.
This latter point does not appear to have been recognized in the original papers on this subject, see [133]. An example of a transversely isotropic material for which \(v_{2}=\overline{v_{1}}\in\mathbb{C}\) is zinc with (all in GPa) \(K=80\), \(\ell=33\), \(n=50\), \(m=63\), \(g=40\), for which \(v_{1}=1.1284+0.6465 i\) to 4dp. (Private communication with P.J. Withers and T. Mori.)
- 2.
This material is Lead Zirconate Titanate, a material frequently used in piezoelectric composites
Notes
Acknowledgements
The author is grateful to the Engineering and Physical Sciences Research Council for funding his research fellowship (EP/L018039/1). He is also thankful to Prof. J. Berger (Colorado School of Mines) and Prof. H. Ammari (ETH, Zurich) for helpful comments.
References
- 1.Ammari, H., Kang, H.: Polarization and Moment Tensors. with Applications to Inverse Problems and Effective Medium Theory. Springer, Berlin (2000) MATHGoogle Scholar
- 2.Ammari, H., Kang, H., Nakamura, G., Tamura, K.: Complete asymptotic expansions of solutions of the system of elastostatics in the presence of an inclusion of small diameter and detection of an inclusion. J. Elast. 67, 97–129 (2003) MathSciNetMATHCrossRefGoogle Scholar
- 3.Ammari, H., Kang, H., Lim, M.: Effective parameters of elastic composites. Indiana Univ. Math. J. 55, 903–922 (2006) MathSciNetMATHCrossRefGoogle Scholar
- 4.Ammari, H., Capdeboscq, Y., Kang, H., Lee, H., Milton, G.W., Zribi, H.: Progress on the strong Eshelby’s conjecture and extremal structures for the elastic moment tensor. J. Math. Pures Appl. 94, 93–106 (2010) MathSciNetMATHCrossRefGoogle Scholar
- 5.Ammari, H., Kang, H., Lee, H., Lim, M.: Enhancement of near cloaking using generalized polarization tensors vanishing structures. Part I: the conductivity problem. Commun. Math. Phys. 317, 253–266 (2013) ADSMathSciNetMATHCrossRefGoogle Scholar
- 6.Asaro, R.J., Barnett, D.M.: The non-uniform transformation strain problem for an anisotropic ellipsoidal inclusion. J. Mech. Phys. Solids 23, 77–83 (1975) ADSMATHCrossRefGoogle Scholar
- 7.Auld, B.A.: Acoustic Fields and Waves in Solids. Krieger, Melbourne (1990) Google Scholar
- 8.Bacon, D.J., Barnett, D.M., Scattergood, R.O.: Anisotropic continuum theory of lattice defects. Prog. Mater. Sci. 23, 51–262 (1980) ADSCrossRefGoogle Scholar
- 9.Barthélémy, J.-F.: Compliance and Hill polarization tensor of a crack in an anisotropic matrix. Int. J. Solids Struct. 46, 4064–4072 (2009) MATHCrossRefGoogle Scholar
- 10.Barthélémy, J.-F.: Effective permeability of media with a dense network of long and micro fractures. Transp. Porous Media 76, 153–178 (2009) MathSciNetCrossRefGoogle Scholar
- 11.Berryman, J.G.: Generalization of Eshelby’s formula for a single ellipsoidal elastic inclusion to poroelasticity and thermoelasticity. Phys. Rev. Lett. 79, 1142–1145 (1997) ADSCrossRefGoogle Scholar
- 12.Bigoni, D., Movchan, A.B.: Statics and dynamics of structural interfaces in elasticity. Int. J. Solids Struct. 39, 4843–4865 (2002) MATHCrossRefGoogle Scholar
- 13.Bond, W.L.: The mathematics of physical properties of crystals. Bell Syst. Tech. J. 22, 1–72 (1943) MathSciNetCrossRefGoogle Scholar
- 14.Buryachenko, V.: Micromechanics of Heterogeneous Materials. Springer, New York (2007) MATHCrossRefGoogle Scholar
- 15.Buryachenko, V., Brun, M.: FEA in elasticity of random structure composites reinforced by heterogeneities of non canonical shape. Int. J. Solids Struct. 48, 719–728 (2011) MATHCrossRefGoogle Scholar
- 16.Buryachenko, V., Brun, M.: Iteration method in linear elasticity of random structure composites containing heterogeneities of non canonical shape. Int. J. Solids Struct. 50, 1130–1140 (2013) CrossRefGoogle Scholar
- 17.Calvo-Jurado, C., Parnell, W.J.: Hashin-Shtrikman bounds on the effective thermal conductivity of a transversely isotropic two-phase composite material. J. Math. Chem. 53, 828–843 (2014) MathSciNetMATHCrossRefGoogle Scholar
- 18.Chen, F., Giraud, A., Sevostianov, I., Dragan, G.: Numerical evaluation of the Eshelby tensor for a concave superspherical inclusion. Int. J. Eng. Sci. 93, 51–58 (2015) CrossRefGoogle Scholar
- 19.Cheng, Z.Q., Batra, R.C.: Exact Eshelby tensor for a dynamic circular cylindrical inclusion. J. Appl. Mech. ASME 66, 563–565 (1999) ADSCrossRefGoogle Scholar
- 20.Cheng, Z.-Q., He, L.-H.: Micropolar elastic fields due to a spherical inclusion. Int. J. Eng. Sci. 33, 389–397 (1995) MathSciNetMATHCrossRefGoogle Scholar
- 21.Cheng, Z.-Q., He, L.-H.: Micropolar elastic fields due to a circular cylindrical inclusions. Int. J. Eng. Sci. 35, 659–668 (1997) ADSMathSciNetMATHCrossRefGoogle Scholar
- 22.Cherepanov, G.P.: Inverse problems of the plate theory of elasticity. J. Appl. Math. Mech. 38, 963–979 (1974) MathSciNetCrossRefGoogle Scholar
- 23.Christensen, R.M., Lo, K.H.: Solutions for effective shear properties in three phase sphere and cylinder models. J. Mech. Phys. Solids 27, 315–330 (1979) ADSMATHCrossRefGoogle Scholar
- 24.Dive, P.: Attraction des ellipsoides homogénes et réciproques d’un théorème de Newton. Bull. Soc. Math. Fr. 59, 128–140 (1931) MathSciNetMATHGoogle Scholar
- 25.Duan, H.L., Wang, J., Huang, Z.P., Karihaloo, B.L.: Eshelby formalism for nano-inhomogeneities. Proc. R. Soc. A 461, 3335–3353 (2005) ADSMathSciNetMATHCrossRefGoogle Scholar
- 26.Dunn, M.L., Taya, M.: Micromechanics predictions of the effective electroelastic moduli of piezoelectric composites. Int. J. Solids Struct. 30, 161–175 (1993) MATHCrossRefGoogle Scholar
- 27.Dunn, M.L., Wienecke, H.A.: Inclusions and inhomogeneities in transversely isotropic piezoelectric solids. Int. J. Solids Struct. 34, 3571–3582 (1997) MATHCrossRefGoogle Scholar
- 28.Dvorak, G.: Micromechanics of Composite Materials. Springer, Berlin (2013) CrossRefGoogle Scholar
- 29.Edwards, R.H.: Stress concentrations around spheroidal inclusions and cavities. J. Appl. Mech. 18, 19–30 (1951) MathSciNetMATHGoogle Scholar
- 30.Eringen, A.C.: Microcontinuum Field Theories I: Foundations and Solids. Springer, New York (1999) MATHCrossRefGoogle Scholar
- 31.Eshelby, J.D.: The determination of the elastic field of an ellipsoidal inclusion, and related problems. Proc. R. Soc. A 241, 376–396 (1957) ADSMathSciNetMATHCrossRefGoogle Scholar
- 32.Eshelby, J.D.: Elastic inclusions and inhomogeneities. In: Sneddon, I.N., Hill, R. (eds.) Progress in Solid Mechanics, vol. 2, pp. 87–140. North-Holland, The Netherlands (1961) Google Scholar
- 33.Franciosi, P.: On the modified green operator integral for polygonal, polyhedral and other non-ellipsoidal inclusions. Int. J. Solids Struct. 42, 3509–3531 (2005) MATHCrossRefGoogle Scholar
- 34.Franciosi, P.: The boundary-due terms in the Green operator of inclusion patterns from distant to contact and to connected situations using Radon transforms: illustration for spheroid alignments in isotropic media. Int. J. Solids Struct. 47, 304–319 (2010) MathSciNetMATHCrossRefGoogle Scholar
- 35.Franciosi, P., Lormand, G.: Using the Radon transform to solve inclusion problems in elasticity. Int. J. Solids Struct. 41, 585–606 (2004) MATHCrossRefGoogle Scholar
- 36.Fritzen, F., Forest, S., Böhlke, T., Kondo, D., Kanit, T.: Computational homogenization of elasto-plastic porous metals. Int. J. Plast. 29, 102–119 (2012) CrossRefGoogle Scholar
- 37.Gao, Z.: A circular inclusion with imperfect interface: Eshelby’s tensor and related problems. J. Appl. Mech. 62, 860–866 (1995) ADSMATHCrossRefGoogle Scholar
- 38.Gao, X.-L., Ma, H.M.: Green’s function and Eshelby’s tensor based on a simplified strain gradient elasticity theory. Acta Mech. 207, 163–181 (2009) MATHCrossRefGoogle Scholar
- 39.Gao, X.-L., Ma, H.M.: Strain gradient solution for Eshelby’s ellipsoidal inclusion problem. Proc. R. Soc. A 466, 20090631 (2010) MathSciNetMATHCrossRefGoogle Scholar
- 40.Gavazzi, A.C., Lagoudas, D.C.: On the numerical evaluation of Eshelby’s tensor and its application to elastoplastic fibrous composites. Comput. Mech. 7, 13–19 (1990) CrossRefGoogle Scholar
- 41.Giordano, S., Palla, P.L., Colombo, L.: Nonlinear elastic Landau coefficients in heterogeneous materials. Europhys. Lett. 83, 66003 (2008) ADSCrossRefGoogle Scholar
- 42.Giraud, A., Huynh, Q.V., Hoxha, D., Kondo, D.: Application of results on Eshelby tensor to the determination of effective poroelastic properties of anisotropic rocks-like composites. Int. J. Solids Struct. 44, 3756–3772 (2007) MATHCrossRefGoogle Scholar
- 43.Goodier, J.N.: Concentration of stress around spherical and cylindrical inclusions and flaws. J. Appl. Mech. 55, 39–44 (1933) Google Scholar
- 44.Gruescu, C., Montchiet, V., Kondo, D.: Eshelby tensor for a crack in an orthotropic elastic medium. C. R., Méc. 333, 467–473 (2005) MATHCrossRefGoogle Scholar
- 45.Hashin, Z.: Theory of mechanical behaviour of heterogeneous solids. Appl. Mech. Rev. 17, 1–9 (1963) Google Scholar
- 46.Hatta, H., Taya, M.: Thermal conductivity of coated filler composites. J. Appl. Phys. 59, 1851–1860 (1986) ADSCrossRefGoogle Scholar
- 47.Hill, R.: A self-consistent mechanics of composite materials. J. Mech. Phys. Solids 13, 213–222 (1965) ADSCrossRefGoogle Scholar
- 48.Hoenig, A.: Elastic moduli of a non-randomly cracked body. Int. J. Solids Struct. 15, 137–154 (1979) MATHCrossRefGoogle Scholar
- 49.Hoenig, A.: Thermal conductivities of a cracked solid. J. Compos. Mater. 17, 231–237 (1983) ADSCrossRefGoogle Scholar
- 50.Hori, M., Nemat-Nasser, S.: Double-inclusion model and overall moduli of multi-phase composites. Mech. Mater. 14, 189–206 (1993) CrossRefGoogle Scholar
- 51.Hu, G.K., Weng, G.J.: The connections between the double-inclusion model and the Ponte-Castaneda–Willis, Mori–Tanaka, and Kuster–Töksoz models. Mech. Mater. 32, 495–503 (2000) CrossRefGoogle Scholar
- 52.Jiang, C.P., Tong, Z.H., Cheung, Y.K.: A generalized self-consistent method accounting for fiber section shape. Int. J. Solids Struct. 40, 2589–2609 (2003) MATHCrossRefGoogle Scholar
- 53.Ju, J.W., Sun, L.Z.: Effective elastoplastic behavior of metal matrix composites containing randomly located aligned spheroidal inhomogeneities. Part I micromechanics based formulation. Int. J. Solids Struct. 38, 183–201 (2001) MATHCrossRefGoogle Scholar
- 54.Kanaun, S.K., Levin, V.M.: Self-Consistent Methods for Composites. Static Problems, vol. 2. Springer, Dordrecht (2008) MATHGoogle Scholar
- 55.Kang, H.: Conjectures of Pólya-Szegö and Eshelby, and the Newtonian potential problem: a review. Mech. Mater. 41, 405–410 (2009) CrossRefGoogle Scholar
- 56.Kang, H., Milton, G.W.: Solutions to the Pólya-Szegö conjecture and the weak Eshelby conjecture. Arch. Ration. Mech. Anal. 188, 93–116 (2008) MathSciNetMATHCrossRefGoogle Scholar
- 57.Kawashita, M., Nozaki, H.: Esehlby tensor of a polygonal inclusion and its special properties. J. Elast. 64, 71–84 (2001) MathSciNetMATHCrossRefGoogle Scholar
- 58.Kellogg, O.D.: Foundations of Potential Theory. Ungar, New York (1970) MATHGoogle Scholar
- 59.Kim, C.I., Schiavone, P.: Designing an inhomogeneity with uniform interior stress in finite plane elastostatics. Int. J. Non-Linear Mech. 197, 285–299 (2007) MATHGoogle Scholar
- 60.Kim, C.I., Vasudevan, M., Schiavone, P.: Eshelby’s conjecture in finite plane elastostatics. Q. J. Mech. Appl. Math. 61, 63–73 (2008) MathSciNetMATHCrossRefGoogle Scholar
- 61.Kinoshita, N., Mura, T.: Elastic fields of inclusions in anisotropic media. Phys. Status Solidi (a) 5, 759–768 (1971) ADSCrossRefGoogle Scholar
- 62.Laws, N.: The determination of stress and strain concentrations at an ellipsoidal inclusion in an anisotropic material. J. Elast. 7(1), 91–97 (1977) MathSciNetMATHCrossRefGoogle Scholar
- 63.Le Quang, H., Bonnet, G., He, Q.-C.: Size-dependent Eshelby tensor fields and effective conductivity of composites made of anisotropic phases with highly conducting interfaces. Phys. Rev. B 81, 064203 (2010) ADSCrossRefGoogle Scholar
- 64.Lee, H.K., Simunovic, S.: A damage constitutive model of progressive debonding in aligned discontinuous fiber composites. Int. J. Solids Struct. 38, 875–895 (2001) MATHCrossRefGoogle Scholar
- 65.Levin, V.M., Alvarez-Tostado, J.M.: Eshelby’s formula for an ellipsoid elastic inclusion in anisotropic poroelasticity and thermoelasticity. Int. J. Fract. 119, 77–82 (2003) CrossRefGoogle Scholar
- 66.Li, J.Y., Dunn, M.L.: Anisotropic coupled-field inclusion and inhomogeneity problems. Philos. Mag. A 77, 1341–1350 (1998) ADSCrossRefGoogle Scholar
- 67.Li, S., Wang, G.: Introduction to Micromechanics and Nanomechanics. World Scientific, Singapore (2008) MATHCrossRefGoogle Scholar
- 68.Li, S., Sauer, R.A., Wang, G.: The Eshelby tensors in a finite spherical domain—Part I: theoretical formulations. J. Appl. Mech. 74, 770–783 (2007) ADSMathSciNetCrossRefGoogle Scholar
- 69.Li, S., Wang, G., Sauer, R.A.: The Eshelby tensors in a finite spherical domain—Part II: applications to homogenization. J. Appl. Mech. 74, 784–797 (2007) ADSMathSciNetCrossRefGoogle Scholar
- 70.Lin, S.C., Mura, T.: Elastic fields of inclusions in anisotropic media (ii). Phys. Solid State A 15, 281–285 (1973) ADSCrossRefGoogle Scholar
- 71.Liu, L.P.: Solutions to the Eshelby conjectures. Proc. R. Soc. A 464, 573–594 (2008) ADSMathSciNetMATHCrossRefGoogle Scholar
- 72.Liu, L.: Solutions to the periodic Eshelby inclusion problem in two dimensions. Math. Mech. Solids 15, 557–590 (2009) MathSciNetMATHCrossRefGoogle Scholar
- 73.Liu, L., James, R.D., Leo, P.H.: Periodic inclusion–matrix microstructures with constant field inclusions. Metall. Trans. A 38, 781–787 (2007) CrossRefGoogle Scholar
- 74.Lubarda, V.A., Markenscoff, X.: On the absence of Eshelby property for non-ellipsoidal inclusions. Int. J. Solids Struct. 35, 3405–3411 (1998) MathSciNetMATHCrossRefGoogle Scholar
- 75.Luo, H.A., Weng, G.J.: On Eshelby’s inclusion problem in a three-phase spherically concentric solid, and a modification of Mori-Tanaka’s method. Mech. Mater. 6, 347–361 (1987) CrossRefGoogle Scholar
- 76.Luo, H.A., Weng, G.J.: On Eshelby’s S-tensor in a three-phase cylindrically concentric solid, and the elastic moduli of fiber-reinforced composites. Mech. Mater. 8, 77–88 (1989) CrossRefGoogle Scholar
- 77.Ma, H., Hu, G.: Eshely tensors for an ellipsoidal inclusion in a micropolar material. Int. J. Eng. Sci. 44, 595–605 (2006) CrossRefGoogle Scholar
- 78.Ma, H., Hu, G.: Eshelby tensors for an ellipsoidal inclusion in a microstretch material. Int. J. Eng. Sci. 44, 3049–3061 (2007) MATHGoogle Scholar
- 79.Markenscoff, X.: Inclusions with constant eigenstress. J. Mech. Phys. Solids 46, 2297–2301 (1998) ADSMathSciNetMATHCrossRefGoogle Scholar
- 80.Markenscoff, X.: On the shape of the Eshelby inclusions. J. Elast. 49, 163–166 (1998) MathSciNetMATHCrossRefGoogle Scholar
- 81.Markov, K.: Elementary micromechanics of heterogeneous media. In: Markov, K., Preziosi, L. (eds.) Heterogeneous Media. Micromechanics Modeling. Methods and Simulations, pp. 1–162. Birkhäuser, Boston (2000). Chap. 1 Google Scholar
- 82.Masson, R.: New explicit expressions of the Hill polarization tensor for general anisotropic elastic solids. Int. J. Solids Struct. 45(3), 757–769 (2008) MATHCrossRefGoogle Scholar
- 83.Maxwell, J.C.: A Treatise on Electricity and Magnetism, vols. 1 and 2. Oxford University Press, Oxford (1998) MATHGoogle Scholar
- 84.Michelitsch, T.M., Gao, H., Levin, V.M.: Dynamic Eshelby tensor and potentials for ellipsoidal inclusions. Proc. R. Soc. A 459, 863–890 (2003) ADSMathSciNetMATHCrossRefGoogle Scholar
- 85.Mikata, Y.: Determination of piezoelectric Eshelby tensor in transversely isotropic piezoelectric solids. Int. J. Eng. Sci. 38, 605–641 (2000) MathSciNetMATHCrossRefGoogle Scholar
- 86.Mikata, Y.: Explicit determination of piezoelectric Eshelby tensors for a spheroidal inclusion. Int. J. Solids Struct. 38, 7045–7063 (2001) MATHCrossRefGoogle Scholar
- 87.Mikata, Y., Nemat-Nasser, S.: Elastic field due to a dynamically transforming spherical inclusion. Int. J. Solids Struct. 38, 7045–7063 (1990) MATHCrossRefGoogle Scholar
- 88.Mikata, Y., Nemat-Nasser, S.: Interaction of a harmonic wave with a dynamically transforming inhomogeneity. J. Appl. Phys. 70, 2071–2078 (1991) ADSCrossRefGoogle Scholar
- 89.Milton, G.W., Serkov, S.K.: Coated inclusions in conductivity and anti-plane elasticity. Proc. R. Soc. A 457, 1973–1999 (2001) ADSMathSciNetMATHCrossRefGoogle Scholar
- 90.Moekher, M.: Fourth-order Cartesian tensors: old and new facts, notions and applications. Q. J. Mech. Appl. Math. 61, 181–203 (2008) MathSciNetCrossRefGoogle Scholar
- 91.Moschovidis, Z.A., Mura, T.: Two-ellipsoidal inhomogeneities by the equivalent inclusion method. J. Appl. Mech. 42, 847–852 (1975) ADSMATHCrossRefGoogle Scholar
- 92.Mura, T.: Micromechanics of Defects in Solids. Kluwer, Hague (1982) CrossRefGoogle Scholar
- 93.Mura, T.: The determination of the elastic field of a polygonal star shaped inclusion. Mech. Res. Commun. 24, 473–482 (1997) MathSciNetMATHCrossRefGoogle Scholar
- 94.Mura, T., Shojda, H.M., Lin, T.Y., Makkawy, A.: The determination of the elastic field of a pentagonal star shaped inclusion. Bull. Tech. Univ. Istanb. 47, 267–280 (1994) MATHGoogle Scholar
- 95.Mura, T., Shodja, H.M., Hirose, Y.: Inclusion problems. Appl. Mech. Rev. 49, S118–S127 (1996) ADSCrossRefGoogle Scholar
- 96.Nguyen, S.T., Dormieux, L., Le Pape, Y., Sanahuja, J.: A Burger model for the effective behavior of a microcracked viscoelastic solid. Int. J. Damage Mech. 20, 1116–1129 (2011) CrossRefGoogle Scholar
- 97.Nikliborc, W.: Eine bemerkung über die Volumpotentiale. Math. Z. 35, 625–631 (1932) MathSciNetMATHCrossRefGoogle Scholar
- 98.Nozaki, H., Taya, M.: Elastic fields in a polygon-shaped inclusion with uniform eigenstrains. J. Appl. Mech. 64, 495–502 (1997) ADSMATHCrossRefGoogle Scholar
- 99.Onaka, S.: Averaged Eshelby tensor and elastic strain energy of a superspherical inclusion with uniform eigenstrains. Philos. Mag. Lett. 81, 265–272 (2001) ADSCrossRefGoogle Scholar
- 100.Onaka, S.: Elastic states of doughnut-like inclusions with uniform eigenstrains treated by averaged Eshelby tensors. Philos. Mag. Lett. 82, 1–7 (2002) ADSCrossRefGoogle Scholar
- 101.Pan, Y.-C., Chou, T.-W.: Point force solution for an infinite transversely isotropic solid. J. Appl. Mech. 43, 608–612 (1976) ADSMATHCrossRefGoogle Scholar
- 102.Parnell, W.J., Calvo-Jurado, C.: On the computation of the Hashin-Shtrikman bounds for transversely isotropic two-phase linear elastic fibre-reinforced composites. J. Eng. Math. 95, 295–323 (2015) MathSciNetMATHCrossRefGoogle Scholar
- 103.Poisson, S.D.: Second mémoire sur la théorie de magnetisme. Mém. Acad. Sci. Inst. Fr. 5, 488–533 (1826) Google Scholar
- 104.Pólya, G., Szegö, G.: Isoperimetric Inequalities for Polarization and Virtual Mass. 21 of Annals of Mathematical Studies. Princeton University Press, Princeton (1951) MATHGoogle Scholar
- 105.Ponte Castañeda, P., Willis, J.R.: The effect of spatial distribution on the effective behaviour of composite materials and cracked media. J. Mech. Phys. Solids 43, 1919–1951 (1995) MathSciNetMATHCrossRefGoogle Scholar
- 106.Qu, J., Cherkaoui, M.: Fundamentals of Micromechanics of Solids. Wiley, New York (2006) CrossRefGoogle Scholar
- 107.Robinson, K.: Elastic energy of an ellipsoidal inclusion in an infinite solid. J. Appl. Phys. 22, 1045–1054 (1951) ADSMathSciNetMATHCrossRefGoogle Scholar
- 108.Rodin, G.J.: Eshelby’s inclusion problem for polygons and polyhedra. J. Mech. Phys. Solids 44, 1977–1995 (1996) ADSCrossRefGoogle Scholar
- 109.Ru, C.Q.: Interface design of neutral elastic inclusions. Int. J. Solids Struct. 35, 559–572 (1998) MATHCrossRefGoogle Scholar
- 110.Ru, C.Q.: Analytic solution for Eshelby’s problem of an inclusion of arbitrary shape in a plane or half-plane. J. Appl. Mech. 66, 315–322 (1999) ADSMathSciNetCrossRefGoogle Scholar
- 111.Ru, C.Q., Schiavone, P.: On the elliptic inclusion in anti-plane shear. Math. Mech. Solids 1, 327–333 (1996) MathSciNetMATHCrossRefGoogle Scholar
- 112.Ru, C.Q., Schiavone, P., Sudak, L.J., Mioduchowski, A.: Uniformity of stresses inside an elliptic inclusion in finite plane elastostatics. Int. J. Non-Linear Mech. 40, 281–287 (2005) ADSMathSciNetMATHCrossRefGoogle Scholar
- 113.Sadowsky, M.A., Sternberg, E.: Stress concentration around an ellipsoidal cavity in an infinite body under arbitrary plane stress perpendicular to the axis of revolution of cavity. J. Appl. Mech. 14, 1947 (1947) MathSciNetMATHGoogle Scholar
- 114.Sadowsky, M.A., Sternberg, E.: Stress concentration around a triaxial ellipsoidal cavity. J. Appl. Mech. 16(2), 149–157 (1949) MathSciNetMATHGoogle Scholar
- 115.Sendeckyj, G.P.: Elastic inclusion problems in plane elastostatics. Int. J. Solids Struct. 6, 1535–1543 (1970) MATHCrossRefGoogle Scholar
- 116.Sevostianov, I., Yilmaz, N., Kushch, V., Levin, V.: Effective elastic properties of matrix composites with transversely-isotropic phases. Int. J. Solids Struct. 42, 455–476 (2005) MATHCrossRefGoogle Scholar
- 117.Sharma, P., Ganti, S.: Size-dependent Eshelby’s tensor for embedded nano-inclusions incorporating surface/interface. J. Appl. Mech. 71, 663–671 (2004) ADSMATHCrossRefGoogle Scholar
- 118.Southwell, R.V., Gough VI, H.J.: On the concentration of stress in the neighbourhood of a small spherical flaw; and on the propagation of fatigue fractures in “Statistically Isotropic” materials. Lond. Edinb. Dublin Philos. Mag. J. Sci. 1(1), 71–97 (1926) CrossRefGoogle Scholar
- 119.Superspheres, S.O.: Intermediate shapes between spheres and polyhedra. Symmetry 4, 336–343 (2012) MathSciNetCrossRefGoogle Scholar
- 120.Suvarov, A.P., Dvorak, G.J.: Rate form of the Eshelby and Hill tensors. Int. J. Solids Struct. 39, 5659–5678 (2002) MATHCrossRefGoogle Scholar
- 121.Walpole, L.J.: The elastic field of an inclusion in an anisotropic medium. Proc. R. Soc. A 300, 270–289 (1967) ADSMATHCrossRefGoogle Scholar
- 122.Walpole, L.J.: The determination of the elastic field of an ellipsoidal inclusion in an anisotropic medium. Math. Proc. Camb. Philos. Soc. 81, 283–289 (1977) MathSciNetMATHCrossRefGoogle Scholar
- 123.Walpole, L.J.: Elastic behaviour of composite materials: theoretical foundations. Adv. Appl. Math. Mech. 21, 169–242 (1981) MATHCrossRefGoogle Scholar
- 124.Walpole, L.J.: Fourth-rank tensor of the thirty-two crystal classes: multiplication tables. Proc. R. Soc. A 391, 149–179 (1984) ADSMathSciNetMATHCrossRefGoogle Scholar
- 125.Wang, Y.M., Weng, G.J.: The influence of inclusion shape on the overall viscoelastic behavior of composites. J. Appl. Mech. 59, 510–518 (1992) ADSMATHCrossRefGoogle Scholar
- 126.Wang, M.Z., Xu, B.X.: The arithmetic mean theorem of Eshelby tensor for a rotational symmetrical inclusion. J. Elast. 77, 13–23 (2004) MathSciNetMATHCrossRefGoogle Scholar
- 127.Weng, G.J.: Some elastic properties of reinforced solids, with special reference to isotropic ones containing spherical inclusions. Int. J. Eng. Sci. 22, 845–856 (1984) MATHCrossRefGoogle Scholar
- 128.Weng, G.J.: Explicit evaluation of Willis’ bounds with ellipsoidal inclusions. Int. J. Eng. Sci. 30, 83–92 (1992) MathSciNetMATHCrossRefGoogle Scholar
- 129.Willis, J.R.: Anisotropic elastic inclusion problems. Q. J. Mech. Appl. Math. 17, 157–174 (1964) MathSciNetMATHCrossRefGoogle Scholar
- 130.Willis, J.R.: Bounds and self-consistent estimates for the overall moduli of anisotropic composites. J. Mech. Phys. Solids 25, 185–202 (1977) ADSMATHCrossRefGoogle Scholar
- 131.Willis, J.R.: A polarization approach to the scattering of elastic waves—I. Scattering by a single inclusion. J. Mech. Phys. Solids 28, 287–305 (1980) ADSMathSciNetMATHCrossRefGoogle Scholar
- 132.Willis, J.R.: Variational and related methods for the overall properties of composites. Adv. Appl. Math. Mech. 21, 1–78 (1981) MathSciNetMATHCrossRefGoogle Scholar
- 133.Withers, P.J.: The determination of the elastic field of an ellipsoidal inclusion in a transversely isotropic medium, and its relevance to composite materials. Philos. Mag. A 59, 759–781 (1989) ADSCrossRefGoogle Scholar
- 134.Wu, T.T.: On the effect of inclusion shape on the elastic moduli of a two-phase material. Int. J. Solids Struct. 2, 1–8 (1966) CrossRefGoogle Scholar
- 135.Yavari, A., Goriely, A.: Nonlinear elastic inclusions in isotropic solids. Proc. R. Soc. A 469, 20130415 (2013) ADSMathSciNetCrossRefGoogle Scholar
- 136.Zhang, Z.K., Soh, A.K.: Micromechanics predictions of the effective moduli of magnetoelectroelastic composite materials. Eur. J. Mech. A, Solids 24, 1054–1067 (2005) ADSMATHCrossRefGoogle Scholar
- 137.Zheng, Q.-S., Zhao, Z.-H., Du, D.X.: Irreducible structure, symmetry and average of Eshelby’s tensor fields in isotropic elasticity. J. Mech. Phys. Solids 54, 368–383 (2006) ADSMathSciNetMATHCrossRefGoogle Scholar
- 138.Zhou, K., Keer, L.M., Wang, Q.J.: Semi-analytic solution for multiple interacting three-dimensional inhomogeneous inclusions of arbitrary shape in an infinite space. Int. J. Numer. Methods Eng. 87, 617–638 (2011) MATHCrossRefGoogle Scholar
- 139.Zhou, K., Jen Hoh, H., Wang, X., Keer, L.M., Pang, J.H.L., Song, B., Wang, Q.J.: A review of recent works on inclusions. Mech. Mater. 60, 144–158 (2013) CrossRefGoogle Scholar
- 140.Zou, W., He, Q., Huang, M., Zheng, Q.: Eshelby’s problem of non-elliptical inclusions. J. Mech. Phys. Solids 58, 346–372 (2010) ADSMathSciNetMATHCrossRefGoogle Scholar
- 141.Zou, W.-N., Zheng, Q.-S., He, Q.-C.: Solutions to Eshelby’s problems of non-elliptical thermal inclusions and cylindrical elastic inclusions of non-elliptical cross-section. Proc. R. Soc. A 467, 607–626 (2011) ADSMathSciNetMATHCrossRefGoogle Scholar
Copyright information
Open Access This article is distributed under the terms of the Creative Commons Attribution 4.0 International License (http://creativecommons.org/licenses/by/4.0/), which permits unrestricted use, distribution, and reproduction in any medium, provided you give appropriate credit to the original author(s) and the source, provide a link to the Creative Commons license, and indicate if changes were made.